Mechanical Modelling of Pultrusion Process_ 2D and 3D Numerical Approaches

Author
abrhamyairaguilarrodriguez 
Category
Documents

view
22 
download
2
Embed Size (px)
description
Transcript of Mechanical Modelling of Pultrusion Process_ 2D and 3D Numerical Approaches

Appl Compos Mater (2015) 22:99118DOI 10.1007/s1044301493943
Mechanical Modelling of Pultrusion Process: 2D and 3DNumerical Approaches
Ismet Baran Jesper H. Hattel Remko Akkerman Cem C. Tutum
Received: 21 March 2014 / Accepted: 7 April 2014 / Published online: 29 May 2014 Springer Science+Business Media Dordrecht 2014
Abstract The process induced variations such as residual stresses and distortions are a critical issue in pultrusion, since they affect the structural behavior as well as the mechanicalproperties and geometrical precision of the final product. In order to capture and investigatethese variations, a mechanical analysis should be performed. In the present work, the twodimensional (2D) quasistatic plane strain mechanical model for the pultrusion of a thicksquare profile developed by the authors is further improved using generalized plane strainelements. In addition to that, a more advanced 3D thermochemicalmechanical analysis iscarried out using 3D quadratic elements which is a novel application for the numerical modelling of the pultrusion process. It is found that the 2D mechanical models give relativelyreasonable and accurate stress and displacement evolutions in the transverse direction ascompared to the 3D model. Moreover, the generalized plane strain model predicts the longitudinal process induced stresses more similar to the ones calculated in the 3D model ascompared with the plane strain model.
Keywords Pultrusion process Finite element analysis Residual/internal stress Thermosetting resin
I. Baran () J. H. HattelDepartment of Mechanical Engineering, Technical University of Denmark, DK2800, Kgs., Lyngby,Denmarkemail: [email protected]
R. AkkermanFaculty of Engineering Technology, University of Twente, NL7500AE, Enschede, The Netherlands
C. C. TutumDepartment of Electrical and Computer Engineering, Michigan State University, East Lansing, MI, USA

100 Appl Compos Mater (2015) 22:99118
Nomenclature
Degree of cureC0 Critical degree of cure at T = 0 KCT Constant used in the shift factor (f (, T ))C Diffusion constantCpc Specific heat of the compositeCpd Specific heat of the dieE Activation energyEr Instantaneous resin modulusE0r Initial (uncured) resin modulusEr Fully cured resin modulusf (, T ) Shift factor (from kinetics to diffusion region)Htr Total heat of reactionkx1,c, kx2,c, kx3,c Thermal conductivities in the x1, x2 and x3directions,
respectively for the compositekx1,d , kx2,d , kx3,d Thermal conductivities in the x1, x2 and x3directions,
respectively for the die Constant used in the Di Benedetto equationKo Preexponential constantn Order of the cure reaction (kinetic exponent)q Heat source (internal heat generation)c Density of the composited Density of the dier Density of the resinR Universal gas constantRr(, T ) Reaction of curet TimeT Instantaneous temperatureTg Glass transition temperatureTg0 Glass transition temperature of the uncured resinTg Glass transition temperature of the fully cured resinT Difference between the glass transition temperature (Tg)
and the instantaneous temperature (T )TC1 Critical temperature at the onset of the glass transitionTC2 Critical temperature at the completion of the glass tran
sitionu Pulling speedVf Fiber volume fraction
1 Introduction
Pultrusion is a continuous and a cost effective composite manufacturing process in whichconstant cross sectional profiles are produced. While pultrusion machines vary in design,the process is basically the same. Creels of unidirectional (UD) roving provide longitudinaltensile strength in the length of the profile. On the other hand, rows of continuous filamentmat (CFM), woven roving or stitched fabrics provide transverse strength across the widthof the profile. All reinforcements are first fed through the preforming guiders which startshaping the fiber reinforcements into the finished product. These reinforcements are then

Appl Compos Mater (2015) 22:99118 101
pulled into a resin bath being wetted out and subsequently entering the heating die. Theheaters initiate the exothermic reaction process in which the resin is being cured. The solidified and cured profile is advanced via a pulling system to the cutoff saw where it is cut toits final length. A schematic view of the pultrusion process is given in Fig. 1.
The process induced variations such as residual stresses and distortions are a criticalissue in composite manufacturing [16], since they affect the structural behaviour and geometrical precision of the final product. More specifically, the residual stresses can lead tocracking during curing [1]. In order to capture and investigate these variations, a mechanicalanalysis should be performed.
In literature, thermochemical characteristics of the pultrusion process has been investigated numerically and experimentally [718] in which the temperature and degree ofcure distributions inside the heating die were predicted. All these contributions have onlybeen dealing with thermal modelling in which the temperature of the composite initiallyis lagging behind the heaters temperature; nevertheless during the curing it exceeds thedie temperature due to the internal heat generation of the resin [7]. For this purpose, wellknown numerical methods such as the finite difference method (FDM)[710] and the finiteelement method (FEM) [1113] have been utilized. Using these efficient thermochemicalmodels, process optimization studies [1416] as well as reliability analysis [17] have beenperformed. In [18], numerical modelling strategies for the thermochemical simulation ofthe pultrusion were investigated by the authors where the steady state approach was found tobe computationally faster than the transient approach. In addition to these thermochemicalstudies in the literature, stateoftheart models have recently been proposed by the authorsfor the thermochemicalmechanical analysis of the pultrusion [19] in which the thermomechanical aspects including the evolution of the process induced stresses and distortionsin the transverse direction together with the mechanical properties were addressed. In thisnumerical model, a three dimensional (3D) transient thermochemical model is sequentiallycoupled with a 2D quasistatic plane strain mechanical model for the pultrusion processof a unidirectional (UD) fiber reinforced profile by using the FEM. The cure hardeninginstantaneous linear elastic (CHILE) approach [20, 21] was utilized for the resin modulusdevelopment. The proposed 3D/2D approach, which was found to be computationally efficient, provides an increased understanding of the process by evaluating the development ofthe stresses and distortions as well as the mechanical properties during processing. In [22],an integrated modelling of the pultrusion process of a NACA0018 blade profile was carriedout by the authors using the proposed 3D/2D mechanical analysis in [19]. The calculatedresidual stresses were transferred to the subsequent bending simulation of the pultrudedblade profile and the internal stress distribution was evaluated taking the process inducedresidual stresses into account.
3D thermochemicalmechanical analysis of the pultrusion process has not been considered in literature up to now. A novel 3D numerical simulation tool embracing the mechanical
Heating Die Puller Saw
Pulling Direction Fibers
Resin Bath
Fiber Guides
Fig. 1 Schematic view of a pultrusion process

102 Appl Compos Mater (2015) 22:99118
aspects of the pultrusion process is hence being developed in the present work. The temperature and degree of cure distributions at steady state are first calculated using the 3Dtransient thermochemical analysis of a pultruded square product. Afterwards, these profiles are mapped to the 2D and 3D quasistatic mechanical models. The already developed2D plane strain mechanical model in [19] is further improved using generalized plane strainelements. Moreover, 3D quadratic brick elements are used for the 3D model for the calculation of the process induced longitudinal stresses as well as transverse stresses. In the 3Dmechanical model, instead of the cross section of the part which is used in the 2D mechanical model (see Fig. 3 [19]), the entire 3D part is assumed to move along the pulling directionof the process while tracking the corresponding temperature and degree of cure profilescalculated in the 3D thermochemical simulation (see Fig. 4). Using these three differentmechanical models (i.e. 2D plane strain, 2D generalized plane strain and 3D models), theevolution of the transient stresses and distortions are captured and the obtained results arecompared with each other. The general purpose finite element software package ABAQUS[23] is utilized. The CHILE approach, which is a valid pseudoviscoelastic approximationof the linear viscoelasticity [24], is considered for the resin modulus evolution as in [19].
2 Numerical Implementation
2.1 ThermoChemical Model
In the thermochemical analysis, the energy equations are solved in 3D space for the UD pultruded part (Eq. 1) and for the die block (Eq. 2). Here, x3 is the pulling (axial or longitudinal)direction; x1 and x2 are the transverse directions.
cCpc
(T
t+ u T
x3
)= kx1,c
2T
x21
+ kx2,c2T
x22
+ kx3,c2T
x23
+ q (1)
dCpd
(T
t
)= kx1,d
2T
x21
+ kx2,d2T
x22
+ kx3,d2T
x23
(2)
where T is the temperature, t is the time, u is the pulling speed, is the density, Cp isthe specific heat and kx1 , kx2 and kx3 are the thermal conductivities along x1, x2 andx3directions, respectively. The subscripts c and d correspond to composite and die, respectively. Lumped material properties are used and assumed to be constant throughout theprocess [19]. The source term q in Eq. 1 is related to the internal heat generation due to theexothermic resin reaction of the thermosetting epoxy resin and expressed as [11]:
q = (1 Vf )rHtrRr (, T ) (3)
where Htr is the total heat of reaction for the epoxy during the exothermic reaction, r isthe resin density, Vf is the fiber volume fraction, is the degree of cure, and Rr(, T ) isthe reaction of cure which can also be defined as the rate of . Htr is calculated from the

Appl Compos Mater (2015) 22:99118 103
areas under the heat flow rate as a function of time obtained from the differential scanningcalorimetry (DSC) tests. In literature, several kinetic models have been proposed and analyzed to describe the resin curing reactivity [25, 26]. In the present work, the well knownmodified nthorder kinetic model is utilized in which the shift from a kineticsdominated toa diffusiondominated resin reaction near the point of vitrification (i.e. transition from rubbery to glassy state) is taken into account by a diffusion factor f (, T ) [19, 20, 27]. Thecorresponding expression is given as:
Rr(, T ) = ddt
= Ko exp( E
RT
)(1 )n f (, T ) (4)
and
f (, T ) = 11 + exp [C( (C0 + CT T ))] (5)
where Ko is the preexponential constant, E is the activation energy, R is the universal gasconstant and n is the order of reaction (kinetic exponent). C is a diffusion constant, C0is the critical degree of cure at T = 0 K and CT is a constant for the increase in critical with T [20]. Ko, E, and n can be obtained by a curve fitting procedure applied to theexperimental data evaluated using the DSC tests [9].
The transient time integration scheme for the rate of the degree of cure can be derived byusing the chain rule. Using this, the rate of the degree of cure can be expressed as:
d
dt=
t+
x3
dx3
dt=
t+ u
x3(6)
and from Eq. 6, the relation of the resin kinetics equation can be expressed as:
t= Rr(, T ) u
x3(7)
where it is the expression in Eq. 7 used in the 3D transient thermochemical model. Theequations presented above have been solved in a 3D domain by means of inhouse developedroutines implemented into the commercial software package ABAQUS.
2.2 Thermochemicalmechanical Model
The temperature and curedependent instantaneous resin modulus is defined as suggestedin the CHILE approach [20]. The corresponding relation is given as:
Er =
E0r T TC1
E0r +T TC1TC2 TC1 (E
r E0r ) f or TC1 < T < TC2
Er TC2 T (8)
where E0r and Er are the initial (i.e. uncured) and fully cured resin moduli, respectively.
TC1 and TC2 are the critical temperatures at the onset and completion of the glass transition,respectively, T represents the difference between the glass transition temperature (Tg) andthe instantaneous resin temperature, i.e. T = Tg T [20]. The evolution of the Tg with thedegree of cure is modelled by the Di Benedetto equation [28] and expressed as:
Tg Tg0Tg Tg0 =
1 (1 ) (9)where Tg0 and Tg are the glass transition temperatures of uncured and fully cured resin,respectively, is a constant used as fitting parameter.

104 Appl Compos Mater (2015) 22:99118
The instantaneous resin elastic modulus (Er ) is used in the calculation of the effectivemechanical properties as well as the thermal and shrinkage strains of the composite part asreported in [19].For this purpose, the self consistent field micromechanics (SCFM) approachis employed which is a well known and documented method in the literature to predict theeffective mechanical properties of the UD composites [2, 19].
An incremental linear elastic approach is implemented utilizing user defined subroutines in ABAQUS for the calculation of the residual stresses and distortions in 2D and 3Dmechanical analyses of the pultrusion process. As aforementioned, quadratic plane strainand generalized plane strain elements for the 2D analysis and brick elements for the 3Danalysis are employed. The incremental total strain tensor (totij ) is composed of the incre
mental mechanical strain (mechij ), thermal strain (thij ) and chemical strain (
chij ) tensors and
expressed as:
totij = mechij + thij + chij (10)
The incremental stress tensor ij is then calculated using the material Jacobian matrix(J) based on the incremental mechanical strain tensor mechij [23] and the correspondingexpression is given as:
ij = Jmechij (11)The details of the relation between the stress and strain tensors used in the present 2D
finite element implementation can be found in [19]. The extension of the correspondingrelation for the 3D mechanical analysis is presented in Eq. 12.
112233121323
=
J11 J12 J13 0 0 0J21 J22 J23 0 0 0J31 J32 J33 0 0 00 0 0 J44 0 00 0 0 0 J55 00 0 0 0 0 J66
112233121323
mech
(12)
where ij is the incremental shear stress tensor, ij is the incremental shear strain tensor andJij s are the elements of the material Jacobian matrix (J) [23].
3 Model Description
3.1 ThermoChemical Analysis
A 3D thermochemical analysis for the pultrusion of a relatively thick (25.4 mm) squareprofile is carried out in a Eulerian frame. The pultrusion model is taken from similar setups available in the literature [9, 11, 19]. A glass/epoxy is considered for the pultrudedproduct in which the fiber reinforcement orientation is UD along the pulling direction andchrome steel is used for the die. Material properties and the resin kinetic parameters arelisted in Table 1 and Table 2, respectively [9, 19]. Only a quarter of the pultrusion domain,seen in Fig. 2, is modelled due to symmetry. Three heating zones having prescribed settemperatures of 171188188C (see Fig. 2) are defined and the spacing between thesezones is defined as 15 mm [9]. The details of the cross section are also shown in Fig. 2.Perfect thermal contact is assumed at the diepart interface as in [11, 19]. Initially (t = 0),the temperature of all nodes are assigned to ambient temperature (27C) and the degree of

Appl Compos Mater (2015) 22:99118 105
Table 1 Material Properties used in the thermochemical simulation of the pultrusion process [9]
Material [kg/m3] Cp [J/kg K] kx3 [W/m K] kx1 , kx2 [W/m K] Vf
Epoxy resin 1260 1255 0.21 0.21 36.1%
Glass fiber 2560 670 11.4 1.04 63.9%
Steel die 7833 460 40 40 
Table 2 Epoxy resin kinetic parameters [9, 19]
Htr [kJ/kg] K0[1/s] E[kJ/mol] n C C0 CT [1/K]
324 192,000 60 1.69 30 1.5 0.0055
cure of all composite nodes are assigned to 0. For t > 0, the temperature of the compositenodes at the die inlet are set to the resin bath temperature 30 C and the degree of cureto 0, respectively. At the symmetry surfaces adiabatic boundaries are defined in which noheat flow is allowed across the boundaries. The remaining exterior surfaces of the die areexposed to ambient temperature with a convective heat transfer coefficient of 10 W/(m2
K) except for the surfaces located at the heating regions. Similarly, at the post die region,convective boundaries are defined for the exterior surfaces of the pultruded square profile.The heat transfer coefficient utilized in the thermochemical analysis is an overall valuewhich actually accounts for both convective and radiation heat transfer during the postdie cooling of the part. The choice of this value (within the realistic range) is not crucialfor the results of the model. The length of the post die region (Lconv) is determined to be13.7 m for cooling down to the ambient temperature after die exit. To reach steady state,the convergence limits are defined as the maximum temperature and cure degree differencebetween the new time step and the old time step and these are set to 0.001 C and 0.0001,respectively.
38.1
12.7
12.7
Symmetry line
Symmetry line 38.1
TH1 [ C] TH2 [ C] TH3 [ C]
171 188 188
x3 x1
x2
Top
Centerx1
x2
Fig. 2 Schematic view of the pultrusion domain for the pultruded square beam. All dimensions are in mm

106 Appl Compos Mater (2015) 22:99118
3.2 ThermoChemicalMechanical Analysis: 2D Approach
In the 2D approach, the 3D thermochemical model defined in Section 3.1 is coupled witha 2D quasistatic mechanical model. Quadratic plane strain and generalized plane strainelements are utilized separately for a comparison analysis of the process induced stressand distortion evolutions. In this 2D mechanical model, the cross section of the compositeis moved through the pulling direction during the process (Lagrangian frame) meanwhiletracking the corresponding temperature and degree of cure profiles already calculated inthe 3D thermochemical analysis (Eulerian frame). Since the length of the pultruded profileis generally much higher than the cross sectional dimensions, the plain strain assumptionis convenient for the analysis of the pultrusion process [19]. For the mechanical analysis,the die is assumed to be rigid and therefore rigid body surfaces are added at the diepartinterface instead of including the meshing for the whole die as was done in the thermochemical analysis. Between the rigid surfaces and the composite part, a mechanical contactformulation is defined which allows separation due to resin shrinkage at the interface andrestricts any expansion of the composite beyond the tool interface. The friction force atthe contact surfaces is assumed to be zero (sliding condition). A generic view of the planestrain model including the rigid surfaces and the mechanical boundary conditions (BCs) areshown in Fig. 3. The resin parameters used in the CHILE approach for the elastic modulusdevelopment are listed in Table 3.
x3
x1
x2
x1
x2
3D Transient thermochemical analysis (Eulerian frame)
2D plane strain quasistatic mechanical analysis (Lagrangian frame)
Temperature (T)Cure degree ( )
2D cross section
t = 0t = t1
t = t2
t = tendx3 = 0x3 = x31
x3 = x32
x3 = x3end
3D composite part
Rigid bodies
2D plane strain/ generalizedplane strain model
x1
x2
Fig. 3 Representation of the coupling of the 3D Eulerian thermochemical model with the 2D Langrangianplainstrain/generalizedplanestrain mechanical model including the rigid body surfaces and the mechanicalBCs

Appl Compos Mater (2015) 22:99118 107
Table 3 Epoxy resin parameters used in the CHILE approach[19, 20]
TC1[C] TC2[C] E0r [MPa] Er [MPa] Tg0 [C] Tg [C]
45.7 12 3.447 3.447e3 0.4 0 195
3.3 ThermoChemicalMechanical Analysis: 3D Approach
In 3D approach, the development of the process induced stresses and distortions are predicted using a 3D quasistatic mechanical model. In this model, the entire 3D composite partdefined in Section 3.1 is assumed to be advanced through the pulling direction while tracking the mapped thermal and cure history. In other words, a 3D Eulerian thermochemicalmodel is coupled with a 3D quasistatic Lagrangian mechanical model (see Fig. 4). Assimilar to the 2D approach, the die surfaces are modelled as rigid surfaces with a similar mechanical contact formulation defined in Section 3.2. Mechanical symmetry BCs areapplied at the symmetry surface in the x1 and x2directions. There is no applied mechanicalBC in the x3direction, i.e. the part can freely move or rotate in the x3direction. The corresponding process induced stresses and distortions are calculated based on the temperatureand the cure distributions together with the corresponding glass transition temperature (Tg)of the composite part. 3D quadratic brick elements are used in the 3D mechanical analysis.The effective mechanical properties of the pultruded part are calculated using the SCFMapproach as aforementioned.
3D Thermochemical analysis (Eulerian frame)
3D quasistatic mechanical analysis (Lagrangian frame)
Temperature (T)Cure degree ( )
3D moving part
t = 0t = t1
t = t2
t = tend
3D composite part
x3
x1
x2
x3 = 0x3 = x31
x3 = x32
x3 = x3end
x3
x1
x2
Fig. 4 Representation of the coupling of the 3D thermochemical model with the 3D mechanical model

108 Appl Compos Mater (2015) 22:99118
4 Results and Discussions
The temperature and the degree of cure profiles together with Tg at steady state are first calculated in the 3D transient thermochemical analysis for the pultrusion of the square beamdefined in Section 3.1. These results are depicted in Fig. 5 and Fig. 6. When the pultrudedpart enters the heating die, it follows these steady state profiles since pultrusion is a continuous process. The pulling speed is set to 20 cm/min [9, 19]. Here, top and centerdenote the top line and the center line through the whole length of the part, respectively, asalso shown in Fig. 2. It is seen that nonuniform temperature (Fig. 5) and degree of cure(Fig. 6) distributions are obtained. The top cures earlier than the center since it is closerto the die having heaters on top of it (Fig. 2). The maximum temperature at the center ispredicted as approximately 217C which is higher than the heater temperature (i.e. 188C)due to the exothermic internal heat generation of the epoxy resin. Tg crosses the compositetemperature of around 173C for the top and 182C for the center at approximately 1.6 mand 1.8 m from die inlet, respectively [19]. It is seen from Fig. 6 that at the post die region(x3 > 0.915 m) the degree of cure is increased slightly which indicates that the curing stilltakes place after the die exit. This fact was also observed in [8]. The degree of cure at thecenter is calculated to be approximately 0.97 at the end of the process (i.e. x3 = 14.6 m).
The obtained temperature and degree of cure distributions together with Tg are mappedto the 2D and 3D quasistatic mechanical analyses as described in Section 3.2 andSection 3.3. In order to reflect the 3D thermochemicalmechanical behaviour of the process more precisely, the mid section of the composite part is considered since the pultrusionis a continuous process, i.e. there is always existing material inside the heating die duringthe process. The mid section is far away from the end boundaries as seen in Fig. 7 in whicha schematic view of the movement of the 3D part in the pulling direction is also depicted.It should be noted that the tracking of the mid section starts at x3 = 7.3 m and ends atx3 = 7.3 m (end of the process). At x3 = 0 m, the mid section enters the heating die. Thecorresponding mapped temperature and degree of cure distributions at the mid section are
0 5 10 15
0
50
100
150
200
3[m]
Tem
pera
ture
[C
]
Center [19]Top [19]Tgcenter [19]Tgtop [19]
Tg
Pulling distance, x
Fig. 5 The temperature and Tg distributions for center and top at the steady state (3D transient thermochemical approach)

Appl Compos Mater (2015) 22:99118 109
0 2 4 6 8 10 12 14 150
0.2
0.4
0.6
0.8
1
3[m]
Deg
ree
of c
ure
Center [19]Top [19]
Pulling distance, x
Fig. 6 The degree of cure profiles for center and top at the steady state (3D transient thermochemicalapproach)
shown in Fig. 8 and Fig. 9, respectively. It is seen that until the mid section enters the heating die, it is assumed that the temperature remains constant as the resin bath temperature of30C and the material remains uncured, i.e. = 0. After entering the heating die, the midsection starts tracking the calculated thermal and cure history. This shows that the calculation domain for the 3D mechanical analysis is between x3 = 7.3 m and x3 = 7.3 m, onthe other hand this is between x3 = 0 m and x3 = 14.6 m for the 2D mechanical analysis.
The evolution of the transient stresses are obtained using the 2D plane strain, generalizedplane strain and 3D quadratic elements in ABAQUS. These results are depicted in Fig. 10
Fig. 7 Schematic view of the movement of the 3D part in the pulling direction and the positioning of themid section. The sizes of the die and the part are not scaled

110 Appl Compos Mater (2015) 22:99118
10 7.5 5 2.5 0 2.5 5 7.5 10 12.5 15
40
60
80
100
120
140
160
180
200
220
3[m]
Tem
pera
ture
[C
]
Center [19]Top [19]CenterMid sectionTopMid section
Die inlet
2.5 1.5 0.5 0.5 1.5 2.5 3.5 4.5 5.5 6.5 7.5
40
60
80
100
120
140
160
180
200
220
3[m]
Tem
pera
ture
[C
]
Center [19]Top [19]CenterMid sectionTopMid section
Die inlet
Die exit
Pulling distance, x Pulling distance, x
Fig. 8 Mapped temperature distributions for center and top at the mid section of the 3D part (lef t). Thecorresponding zoomed plot of the temperature profiles (right) for the axial distance between 2.5 m and7.5 m
and Fig. 11 for center and top, respectively. Here, S11, S22 and S33 are the normal stressesin the x1direction (horizontal, transverse), the x2direction (vertical, transverse) and the x3direction (longitudinal), respectively. It is seen that the transverse normal stresses are foundto be almost similar using both 2D and 3D approaches in terms of magnitude and evolutiontrend as compared with published data [19]. It is obvious that the 3D mechanical modelis a more advanced and realistic numerical tool as compared to 2D models. Bearing thisin mind, the plane strain assumption for the mechanical analysis of the pultrusion processgives accurate results and is a convenient way of modelling for the prediction of transversestresses. For the 3D mechanical analysis, it is seen that until the mid section enters the die,there is almost no transverse stresses, i.e. S11 and S22 are zero before the die inlet. Thisshows that the already pulled material (e.g. the portion inside the heating die) has almost noeffect on the stress development at the mid section before entering the die. Inside the die,the stress levels are relatively small because the matrix material has not enough stiffness
10 7.5 5 2.5 0 2.5 5 7.5 10 12.5 150
0.2
0.4
0.6
0.8
1
3[m]
Deg
ree
of c
ure
Center [19]Top [19]CenterMid sectionTopMid section
Die inlet
2.5 1.5 0.5 0.5 1.5 2.5 3.5 4.5 5.5 6.5 7.50
0.2
0.4
0.6
0.8
1
3[m]
Deg
ree
of c
ure
Center [19]Top [19]CenterMid sectionTopMid section
Die inlet
Die exit
Pulling distance, x Pulling distance, x
Fig. 9 Mapped degree of cure distributions for center and top at the mid section of the 3D part (lef t). Thecorresponding zoomed plot of the degree of cure profiles (right) for the axial distance between 2.5 m and7.5 m

Appl Compos Mater (2015) 22:99118 111
to build up the stresses. The outer regions closest to the die cure first which make themconstrained by the inner region during shrinkage. Due to this, a residual compression isfound in these regions and tension prevails for the inner regions at the end of the processupholding the self static equilibrium.
Regarding the longitudinal stress development (S33 for center in Fig. 10 and for topin Fig. 11) in the pulling or fiber direction, a different mechanical behaviour is obtainedas compared to the development in the transverse directions (S11 and S22). It is seen thatunrealistic and overestimated transient S33 values are obtained using the plane strain elements. On the other hand more realistic stress values are calculated using the generalizedplane strain elements since outofplane strain is now allowed to take place within certainrestrictions. Therefore, the resulting S33 values obtained by using the generalized planestrain elements are much closer to the values in the 3D mechanical analysis. Although thematrix material is in a liquid state before entering the die (the degree of cure is zero) for the3D mechanical analysis, a nonzero S33 (value of approximately 2 MPa) is found to existat the mid section (center) while entering the die as seen in Fig. 10d. From modelling pointof view, this is due to the stress gradient through the thickness in combination with a low
8 0 4 2 0 2 4 6 8 10 12 14151
0
1
2
3
4
3[m]
S11
[MP
a]
PS [19]GPS3D
Die inlet
Die exit
8 6 4 2 0 2 4 6 8 10 12 14151
0
1
2
3
4
3[m]
S22
[MP
a]
PS [19]GPS3D
Die inlet
Die exit
8 6 4 2 0 2 4 6 8 10 12 141550
40
30
20
10
0
10
20
3[m]
S33
[MP
a]
PSGPS3D
Die exit
Die inlet
8 6 4 2 0 2 4 6 84
2
0
2
4
6
3[m]
S33
[MP
a]
3D
Die inlet
Die exit
ba
dc
Pulling distance, x
Pulling distance, x Pulling distance, x
Pulling distance, x
Fig. 10 The transient stress evolutions at center (S11 (a), S22 (b) and S33 (c)) which are calculated usingthe plane strain (PS), generalized plane strain (GPS) and 3D quadratic brick elements. The zoomed plot ofS33 for 3D elements are depicted in (d)

112 Appl Compos Mater (2015) 22:99118
8 6 4 2 0 2 4 6 8 10 12 1415
12
10
8
6
4
2
0
2
3[m]
S11
[MP
a] PS [19]GPS3D
Die inlet
Die exit
8 6 4 2 0 2 4 6 8 10 12 14150.4
0.3
0.2
0.1
0
0.1
0.2
0.3
0.4
3[m]
S22
[MP
a]
PS [19]GPS3D
Die exit
Die inlet
8 6 4 2 0 2 4 6 8 10 12 141540
30
20
10
0
10
3[m]
S33
[MP
a]
PSGPS3D
Die exitDie inlet
8 6 4 2 0 2 4 6 8
0.25
0.2
0.15
0.1
0.05
0
0.05
0.1
0.15
0.2
3[m]
S33
[MP
a]
3D
Die exitDie inlet
ba
dc
Pulling distance, x
Pulling distance, x Pulling distance, x
Pulling distance, x
Fig. 11 The transient stress evolutions at top (S11 (a), S22 (b) and S33 (c)) which are calculated using theplane strain (PS), generalized plane strain (GPS) and 3D quadratic brick elements. The zoomed plot of S33for 3D elements are depicted in (d)
shear modulus at the liquid state. Nevertheless, it will not appear in practice and the regionbefore die is out of interest in terms of the mechanical variations in the processing material.As mentioned before, this 3D effect is not pronounced in the transverse directions. The longitudinal stress levels (S33) calculated using the generalized plane strain and 3D elementsare found to be relatively small as compared to S11 and S22 since the longitudinal component of the process induced strain is smaller than the transverse component (see Fig. 12 forthe process induced strain development at center). The reason for that is the constrainingfiber stiffness in the pulling direction which was also investigated in [2].
The corresponding contour plots of S11, S22 and S33 at the end of the process are seenin Fig. 13 (plane strain solution), Fig. 14 (generalized plane strain solution) and Fig. 15(3D solution). The stress distributions in the transverse directions (i.e. S11 and S22) overthe cross section of the part have almost the same pattern for these three different types ofanalysis. As expected, the S11 distribution is almost symmetric with the S22 distributionwith respect to the diagonal of the pultruded part, since all the mechanical boundary conditions are the same. The generalized plane strain results (Fig. 14) and the 3D results (Fig. 15)have the similar distribution trend for the S33 distribution, such that tension and compression stresses are found to prevail in the pulling direction. On the other hand, the plane

Appl Compos Mater (2015) 22:99118 113
0 2 4 6 8 10 12 14 154
2
0
2
4
6
8x 10
3
3[m]
Pro
cess
indu
ced
stra
in (
th+
ch) Transverse
Longitudinal
Pulling distance, x
Fig. 12 The process induced strain, which is the summation of the thermal strain (th) and the chemicalshrinkage strain (ch), for center in the transverse and longitudinal direction
Fig. 13 Undeformed contour plots of the normal stresses S11, S22 and S33 calculated using the plane strainelements at the end of the process (x3 = 14.6 m). All units are in Pa

114 Appl Compos Mater (2015) 22:99118
Fig. 14 Undeformed contour plots of the normal stresses S11, S22 and S33 calculated using the generalizedplane strain elements at the end of the process (x3 = 14.6 m). All units are in Pa
strain solution predicts unrealistic S33 values such that the whole cross section is under tension showing that the self static equilibrium in the longitudinal direction is not fulfilled asexpected. The reason for this is that there is no strain in the longitudinal direction for theplane strain assumption. This may not be a valid assumption for the calculation of the S33since there is an existing strain in the pulling direction.
The calculated maximum tension and compression stresses at the end of the process aregiven in Table 4. It is seen that the lowest stress levels are obtained for the 3D mechanicalsolution which is also intuitively expected. The maximum tension stress level is found tobe approximately between 34 MPa and the maximum compression level is approximatelybetween 1216 MPa for S11 and S22. For S33, the levels are approximately between 1.72.5MPa and 3.654.25 MPa, respectively, without considering the plane strain solution since itis overestimating S33.
The evolution of the displacement profile is also predicted using the devised numericalsimulation tools for the top in the x2direction (U2). The results are depicted in Fig. 16.It is found that there is a good match between the U2 evolutions obtained using the threedifferent element types. It should be noted that the initial pressure condition of the partbefore entering the heating die is not taken into account which may affect the stress anddisplacement field.

Appl Compos Mater (2015) 22:99118 115
Fig. 15 Undeformed contour plots of the normal stresses S11, S22 and S33 for the mid section (see Fig. 7)calculated using the 3D elements at the end of the process (x3 = 7.3 m). All units are in Pa
Table 4 The maximum tension and compression stresses predicted at the cross section of the pultrudedproduct using the plane strain (PS), generalized plane strain (GPS) and the 3D elements.
S11 [MPa] S22 [MPa] S33 [MPa]
4.14 (PS) 4.15 (PS) 16.93 (PS)
Max. tension 3.70 (GPS) 3.68 (GPS) 2.54 (GPS)
3.48 (3D) 3.44 (3D) 1.74 (3D)
16.03 (PS) 16.00 (PS)  (PS)
Max. compression 13.69 (GPS) 14.00 (GPS) 4.25 (GPS)
12.81 (3D) 13.48 (3D) 3.65 (3D)

116 Appl Compos Mater (2015) 22:99118
8 6 4 2 0 2 4 6 8 10 12 1415
8
6
4
2
0
x 105
Axial distance, x3
[m]
U2
[m]
PS [19]GPS3D
Die exit
Die inlet
Fig. 16 Displacement evolution for top in the x2direction (U2) calculated using the plane strain (PS),generalized plane strain (GPS) and 3D elements (mid section for the 3D model)
5 Conclusions
In the present work, the 2D quasistatic plane strain mechanical model developed by theauthors for the pultrusion process is further improved using the generalized plane strainelements. In addition, 3D quadratic brick elements are also utilized for the 3D thermochemicalmechanical model for the calculation of the longitudinal stresses which has notbeen considered up to now in the field of numerical modelling of the pultrusion process.The temperature and degree of cure distributions at steady state are first calculated usinga 3D transient thermochemical analysis. Afterwards, these profiles are mapped to the 2Dand 3D quasistatic mechanical models. Using these three different mechanical models (i.e.2D plane strain, 2D generalized plane strain and 3D models), the development of the process induced stresses and distortions are predicted for the pultrusion of a UD glass/epoxysquare profile. The obtained results are compared with each other. The main outcomes aresummarized as follows:
i) It is found that there is a good agreement between the calculated transverse stress evolutions (S11 and S22) together with the transverse displacement profiles (U2) usingthe 2D and 3D mechanical models. This shows that the plane strain assumption is aconvenient and fast way of predicting the transverse stresses and displacements.
ii) For the calculation of the longitudinal stresses (S33), generalized plane strain and3D elements predict more realistic stress values as compared to the plane strainelements in which overestimated S33 values are obtained.
iii) The predicted stress level for S33 is found to be lower than the S11 and S22 since thelongitudinal component of the process induced strain is smaller than the transversecomponent.
iv) Lower stress values are obtained in the 3D mechanical analysis as compared with the2D analyses which is intuitively expected.

Appl Compos Mater (2015) 22:99118 117
The proposed 3D/3D thermochemicalmechanical model is found to be more suitable foradvanced modelling of the pultrusion process, e.g. taking the effect of the frictional forceinside the heating die on the longitudinal process induced stress levels into account. Onthe other hand, the 2D generalized plane strain mechanical model is found to be computationally fast as compared with the 3D model and is therefore more efficient and usefulfor internal stress investigation in the transverse directions of the pultruded products, e.g.the transverse residual stresses at the webflange junctions of pultruded Ibeam profiles ortransverse warpage in pultruded hollow rectangular profiles.
Acknowledgments This work is a part of the DeepWind project which has been granted by the EuropeanCommission (EC) under the FP7 program platform Future Emerging Technology.
References
1. Wisnom, M.R., Gigliotti, M., Ersoy, N., Campbell, M., Potter, K.D.: Mechanisms generating residual
(2006)2. Bogetti, T.A., Gillespie, J.W.: Processinduced stress and deformation in thicksection thermoset
composite laminates. J. Compos. Mater. 26(5), 626660 (1992)3. Ersoy, N., Garstka, T., Potter, K., Wisnom, M.R., Porter, D., Stringer, G.: Modelling of the springin
phenomenon in curved parts made of a thermosetting composite. Compos. Part A 41, 410418 (2010)4. White, S.R., Hahn HT: Process modeling of composite materials:Residual stress development during
cure. Part I. Model formulation. J. Compos. Mater. 26(16), 24022422 (1992a)5. White, S.R., Hahn HT: Process Modeling of Composite Materials:Residual Stress Development during
Cure. Part II. Experimental Validation. J. Compos. Mater. 26(16), 24232453 (1992b)6. Nielsen, M.W., Schmidt, J.W., Hattel, J.H., Andersen, T.L., Markussen, C.M.: In situ measurement using
FBGs of processinduced strains during curing of thick glass/epoxy laminate plate: experimental resultsand numerical modelling. Wind energy 2012.
7. Baran, I., Tutum, C.C., Hattel, J.H.: The effect of thermal contact resistance on the thermosettingpultrusion process. Compos. Part B: Eng. 45, 9951000 (2013)
8. Valliappan, M., Roux, J.A., Vaughan, J.G., Arafat, E.S.: Die and postdie temperature and cure ingraphiteepoxy composites. Compos. Part BEng. 27, 19 (1996)
9. Chachad, Y.R., Roux, J.A., Vaughan, J.G., Arafat, E.: Threedimensional characterization of pultrudedfiberglassepoxy composite materials. J. Reinf. Plast. Comp. 14, 495512 (1995)
10. Ding Z, Li S, Lee LJ.: Influence of heat transfer and curing on the quality of pultruded composites. ii:Modeling and simulation. Polym. Compos. 23, 957969 (2002)
11. Liu, X.L., Crouch, I.G., Lam, Y.C.: Simulation of heat transfer and cure in pultrusion with a generalpurpose finite element package. Compos. Sci. Technol. 60, 857864 (2000)
12. Carlone, P., Palazzo, G.S., Pasquino, R.: Pultrusion manufacturing process development by computational modelling and methods. Math. Comput. Model. 44, 701709 (2006)
13. Suratno, B.R., Ye, L., Mai, Y.W.: Simulation of temperature and curing profiles in pultruded compositerods. Compos. Sci. Technol. 58, 191197 (1998)
14. Carlone, P., Palazzo, G.S.: Pultrusion manufacturing process development:Cure optimization by hybridcomputational methods. Comput. Math. Appl. 53, 14641471 (2007)
15. Baran, I., Tutum, C.C., Hattel, J.H.: Optimization of the thermosetting pultrusion process by using hybridand mixed integer genetic algorithms. App. Compos. Mat. 20, 449463 (2012)
16. Tutum, C.C., Baran, I., Hattel, J.H.: Utilizing multiple objectives for the optimization of the pultrusionprocess. Key Eng. Mater. 554557, 21652174 (2013)
17. Baran, I., Tutum, C.C., Hattel, J.H.: Reliability estimation of the pultrusion process using the firstorderreliability method (FORM). App. Compos. Mat. 20, 639653 (2012)
18. Baran, I., Hattel, J.H., Tutum, C.C.: ThermoChemical modelling strategies for the pultrusion process.App. Compos. Mat. (2013)
19. Baran, I., Tutum, C.C., Nielsen, M.W., Hattel, J.H.: Process induced residual stresses and distortions inpultrusion. Compos. Part B: Eng. 51, 148161 (2013)
stresses and distortion during manufacture of polymermatrix composite structures, Vol. 37, pp. 522529

118 Appl Compos Mater (2015) 22:99118
20. Johnston A.: An integrated model of the development of processinduced deformation in autoclaveprocessing of composites structures, Ph.D. thesis. The University of British Columbia, Vancouver (1997)
21. Nielsen MW: Predictions of process induced shape distortions and residual stresses in large fibre reinforced composite laminates, Ph.D. thesis, deparment of mech. Eng. Technical University of Denmark,Denmark (2012)
22. Baran, I., Tutum, C.C., Hattel, J.H.: The internal stress evaluation of the pultruded blades for a Darrieuswind turbine. Key Eng. Mater. 554557, 21272137 (2013)
23. ABAQUS 6.11 Reference Guide. Dassault Systems (2011)24. Zobeiry, N., Rasekh, A., Vaziri, R., Poursartip, A.: Efficient modelling techniques for predicting process
ing residual stress and deformation in composite parts. Proceedings of the 14th international conferenceon composite materials ICCM14, San Diego, United States of America (2003)
25. Kenny, J.M.: Determination of autocatalytic kinetic model parameters describing thermoset cure. J.Appl. Polym. Sci. 51, 761764 (1994)
26. Kessler, M.R., White, S.R.: Cure kinetics of the ringOpening metathesis polymerization of dicyclopentadiene. J. Poly. Sci. Part A: Poly. Chem. 40, 23732383 (2002)
27. Khoun, L.: Processinduced stresses deformations in woven composites manufactured by resin transfermoulding. Ph.D. Thesis,McGill University, Montreal (2009)
28. Khoun L, Centea T, Hubert P: Characterization methodology of thermoset resins for the processing ofcomposite materials case study: CYCOM 890RTM epoxy resin. J. Compos. Mater. 44, 1397415 (2010)
Mechanical Modelling of Pultrusion Process: 2D and 3D Numerical ApproachesAbstractNomenclatureIntroductionNumerical ImplementationThermoChemical ModelThermochemicalmechanical Model
Model DescriptionThermoChemical AnalysisThermoChemicalMechanical Analysis: 2D ApproachThermoChemicalMechanical Analysis: 3D Approach
Results and DiscussionsConclusionsAcknowledgmentsReferences